A synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks

 Horace Glenn
 9 months ago
 Views:
Transcription
1 Article A synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks JOURNAL OF COMPOSITE MATERIALS Journal of Composite Materials 0(0) 7! The Author(s) 0 Reprints and permissions: sagepub.co.uk/journalspermissions.nav DOI: 0.77/ jcm.sagepub.com Chandra Veer Singh and Ramesh Talreja, Abstract We treat selected test cases in the third world wide failure exercise by the approach described as synergistic damage mechanics. This approach utilizes micromechanics and continuum damage mechanics to predict the overall mechanical response of composite laminates with ply cracking in multiple orientations. The material constants needed in the continuum damage mechanic formulation are calculated from stiffness property changes incurred in a reference laminate. For other laminate configurations, the stiffness changes are derived using a relative constraint parameter which is calculated from the constraint on the opening displacement of ply cracks within the given cracked laminate evaluated numerically by a finite element analysis of appropriately constructed representative unit cell. The number density of ply cracks (cracks per unit length normal to the crack planes) under quasistatic loading is calculated by an energybased approach. Finally, the stress strain response of a laminate is determined by combining stiffness property changes and evolution of crack number density. Keywords Synergistic, continuum damage mechanics, cracks, unit cell Introduction and historical background Failure analysis of composite materials is currently performed by the industry using empirical criteria, none of which properly accounts for the effects of damage processes prior to complete failure. Significant developments in the past three decades suggest that accounting for subcritical damage will improve composite design. While previous exercises, focused on the ultimate failure, the third world wide failure exercise (WWFEIII) provides an opportunity to examine initiation and progression of subcritical events and their effect on the mechanical response. In composite laminates, which are the subject of examination in WWFEIII, the damage initiation processes begin at the constituent level within a ply. In most cases, ply cracks span the thickness and width of the ply at relatively low loads. Subsequent loading then results in multiplication of these cracks. It is common, therefore, to start the analysis with assumed presence of ply cracks and examine their evolution (increase in number per unit length normal to crack planes) as well as the effect of these cracks in changing the laminateaveraged mechanical properties. The approaches taken to address this problem can be broadly characterized as microdamage mechanics (or simply, micromechanics), e.g. shearlag methods, see for example References [4 ], and continuum damage mechanics (CDMs). Our current approach is to retain the framework of CDM but enrich its capabilities by combining it with micromechanics. We have called this approach synergistic damage mechanics (SDM). The present paper will first briefly describe the SDM methodology and then apply it to selected cases of WWFEIII. The CDM 7,8 uses a physically based damage characterization that does not leave behind essential features of damage in the context of the material response of Department of Materials Science and Engineering, University of Toronto, Toronto, ON, Canada Department of Aerospace Engineering, Texas A&M University, College Station, TX, USA Visiting Professor, Luleå University of Technology, Luleå, Sweden Corresponding author: Ramesh Talreja, Department of Aerospace Engineering, Texas A&M University, College Station, TX , USA. Downloaded from jcm.sagepub.com at UNIV TORONTO on January 5, 0
2 Journal of Composite Materials 0(0) interest while keeping in sight practical implementation of the resulting methodology. As argued in References [7,8] and elaborated further in References [9 ], a scalarvalued characterization would be inadequate in view of the oriented nature of the internal surfaces formed. Although a vectorvalued characterization was employed at first, the issue of ambiguity of the sense of a vector could be addressed more elegantly by using a second order tensor instead. The damage characterization for ply cracking involved calculation of a constraint parameter,, which essentially captures the environment of the cracked surfaces (e.g. effect of surrounding plies), and a number of damage constants, c i which depend on the laminate material. These constants will be described later. The observation that the parameter may be viewed as a carrier of the local effects on damage entities within a Representative Volume Element (RVE), while the c i constants are material constants, led to a number of studies to explore prediction of elastic property changes due to damage in different modes. To be sure, the elastic properties are the averages over appropriate RVEs. CDM model considered here predicts effective stiffness changes for the whole laminate; layerwise (or laminawise) CDM model have also been developed., At first it was found that from changes in E x and xy due to transverse cracking in [0/90 ] s glass/epoxy laminates reported in Reference [4] and assuming no changes in E y, changes in E x for the same glass/epoxy of [0/90] s configuration could be predicted with good accuracy. Also, in [0/45] s laminate of the same glass/ epoxy, the change in E x could be predicted by setting damage parameters D(þ45) ¼ D(45) (a good approximation, supported by crack density data). These results have been reported in Reference [9]. Later, a systematic study of the effect of constraint on the constraint parameter was done by experimentally measuring the crack opening displacement (COD) in [/90 ] s laminates 5 7 for different  values. By relating these values to the COD at ¼ 90 and normalized by a unit applied strain, the predictions of E x and xy for different could be made. Another study of the constraint effects was made by examining [0/ 4 / 0/ ] s laminates, where the ply orientation was varied. Once again, using experimentally measured COD for ¼ 90 as the reference, the parameter for other ply orientations was evaluated from the COD values and E x and xy for different were predicted. 8 While the experimental studies supported the idea of using the constraint parameter as a carrier of local constraints, the scatter in test data and the cost of testing do not make the experimental approach attractive. Therefore, another systematic study of [0 m / n /0 m/ ] s laminates was undertaken 9,0 where computational micromechanics was employed instead of physical testing as a means of evaluating the constraint parameter. An elaborate parametric study of the constraint parameter allowed developing a master curve for elastic property predictions. The most recent study examines damage modes consisting of transverse ply cracks as well as inclined cracks of different orientations in [0 m / n /90 r ] s and [0 m /90 r / n ] s laminates. The SDM approach is developed and its predictions are compared with available experimental data for [0/90/45/þ45] s laminate. At the current state of its development, the SDM methodology has the ingredients of a multiscale damage mechanics depicted in Figure. As illustrated there, structural (macroscale) analysis of a part containing damage is accomplished by a mesoscale SDM analysis of appropriate RVE in which microscale input from micromechanics (computed CODs) as well as materials constants from a reference laminate configuration are entered. What remains is to codify this approach in software to be used by design engineers. Theoretical details Definition of damage Consider a continuum body of a composite solid with a matrix and embedded reinforcements as well as a multitude of damage entities in the form of microcracks. In CDM, the material microstructure, e.g., distributed fibres, and the distributed damage, which may be called the microdamage structure, are treated as smearedout fields. For evaluating the effective properties of the continuum body, the continuum is homogenized using a twostep homogenization procedure (see Figure ). As illustrated in the figure, the material microstructure is viewed as consisting of stationary entities, e.g., fibres and plies, and the microdamage structure is considered as a family of evolving entities, e.g., cracks and voids. First the stationary microstructure is smeared into a homogeneous, anisotropic material. In the next step, the evolving microstructure is replaced by a homogeneous field represented by suitable internal variables. The internal microdamage structure evolves with loading and causes changes of the overall response (properties) of the composite. Resorting to Figure again, consider a generic point P inside the damaged composite body. Let an element of volume V contain a representative sample of damage entities about this point. An individual damage entity (a crack or a void) can be viewed as bounded by a surface S, on which any point can be associated with two vectors, one of which, a, represents a selected influence of the damage entity, and the other, n, is the unit outward normal to the surface. Let the surface integral of dyadic product of the vector components a i n j be Downloaded from jcm.sagepub.com at UNIV TORONTO on January 5, 0
3 Singh and Talreja Figure. Multiscale synergistic methodology for analyzing damage behaviour in a general symmetric laminate [0 m / n /90 r ] s with matrix cracks in þ, and 90 layers. Stationary microstructure RVE for damage characterization Evolving microstructure Step Homogenization of stationary microstructure P Step V Homogenization of evolving microstructure P a i n j Continuum after homogenizing the stationary microstructures Fully homogenized continuum Characterization of a damage entity Figure. Homogenization of a continuum body with damage. Downloaded from jcm.sagepub.com at UNIV TORONTO on January 5, 0
4 4 Journal of Composite Materials 0(0) denoted by the secondorder tensor components d ij. Thus, Z d ij ¼ a i n j ds s The total set of damage entities may be divided in subsets of entities having same geometrical characteristics (orientation, shape, etc.) and termed as damage modes. For example, matrix cracks may constitute one damage mode, while fibre/matrix debonds may constitute another. Also, matrix cracks in different orientations may be grouped into different damage modes. Assuming that there are N damage entities of a given mode a in the RVE, the damage mode tensor is defined by D ðþ ij ¼ X V k d ij k where k ¼,,..., N and V is the volume of the RVE. Let us now focus on the particular case of intralaminar cracking in composite laminates. Figure shows an RVE illustrating one set of intralaminar cracks in an offaxis ply of a composite laminate. Although for clarity of illustration, the cracking is shown only in one lamina, it is understood that in general it exists in multiple plies of the laminate. The thickness of the cracked plies is denoted by t c, s is the average crack spacing, t is the total laminate thickness and W and L stand for the width and the length, respectively, of the RVE. The volume of the RVE, the surface area of a crack, S, and the influence vector magnitude, a, are specified as V ¼ L W t S ¼ W t c sin a ¼ t c where, called the constraint parameter, is an unspecified constant of (assumed) proportionality between a and the crack size t c (also crackedply thickness). Here, 0 p/, so that S is always positive. Assuming a to be constant over the crack surface S, one gets from equation () ðþ ðþ ðþ The synergistic damage mechanics methodology For the mechanical response of a damaged body in isothermal condition, the Helmholtz free energy function is given by 9 ¼ " ij, D ðþ Helmholtz free energy is thus a function of the damage state. The energy change brought about by damage is represented by terms involving D ðþ ij. The stress tensor is then given by ij ij ij where m is the mass density. For a linear elastic homogenized body, ij ¼ C ijkl " kl where the stiffness matrix C ijkl is given in the Voigt notation as C pq ¼ C 0 pq þ X C ðþ pq where C 0 pq is the initial (undamaged) stiffness matrix and P C ðþ pq represents the stiffness changes brought about by all the damage modes. In the following, we consider the different cases of cracking in composite laminates and derive the corresponding damagestiffness relations. Case : Only 90 ply is cracked (single damage mode). Let us consider the Helmholtz free energy for a composite laminate with its 90 ply cracked. As shown before, 8 0 a polynomial form is most suited for our formulation. Assuming the composite laminates in consideration to be orthotropic, the form of the polynomial must remain invariant with respect to the coordinate transformations expressing this symmetry. Such restrictions to polynomial functions are satisfied by making use of certain polynomial invariants called the irreducible integrity basis.,4 Considering a single damage mode, ¼, we have the following set of invariants ", ", ", ", ", ", " " " ð5þ ðþ ð7þ ð8þ D ðþ ij ¼ t c st sin n in j where n i ¼ ðsin, cos, 0Þ. ð4þ D, D, D, D, D, D, D D D " D, " D, " D, " " D, " " D, " " D, " D D, " D D, " D D ð9þ Downloaded from jcm.sagepub.com at UNIV TORONTO on January 5, 0
5 Singh and Talreja 5 Figure. A representative volume element illustrating intralaminar multiple cracking in a general offaxis ply of a composite laminate. This set of integrity bases can be further reduced for the case of a thin laminate loaded in its plane. For such laminates, only the inplane transformed strain and damage tensor components need be considered. Thus, the remaining integrity bases in the Voigt notation for thin laminates are given by where ", ", " D, D, D " D ð0þ " "," "," ",D D,D D,D D : The most general polynomial form for Helmholtz free energy, restricted to secondorder terms in the damage strain components and first order terms in damage tensor components (low volume fraction of damage entities), is given by ¼ P 0 þ c " þ c " þ c " þ c 4" " þ c 5 " D þ c " D þ c7 " D þ c 8 " D þ c 9 " D þ c 0 " D þ f c " " D þ c " " D g þ fc " " D þ c 4 " " D gþp ð" p, D q ÞþP ðd q Þ ðþ where P 0 and c i, i ¼,,..., 4 are material constants, P is a linear function of strain and damage tensor components and P is a linear functions of damage tensor components. Setting the free energy to zero for unstrained and undamaged material, we have, P 0 ¼ 0, and assuming the unstrained material of any damaged state to be stressfree, we get P ¼ 0. The stress Downloaded from jcm.sagepub.com at UNIV TORONTO on January 5, 0
6 Journal of Composite Materials 0(0) components in the Voigt notation are now given by (from equation ()) p p where p ¼,,. From () and (), we have where p, q ¼,,, and C pq ¼ C 0 pq þcðþ pq c c 4 0 C 0 pq ¼ c Symm c E 0 0 x xy E0 y 0 xy 0 yx 0 xy 0 yx ¼ E 0 y 0 xy 0 yx 4 Symm 0 0 G 0 xy 7 5 ðþ ðþ ð4þ represents the orthotropic stiffness matrix for virgin composite material, where E 0 x, E0 y, 0 xy, G0 xy are effective moduli for the undamaged laminate (calculated using CLT), and c 5 D þ c D pq ¼ 4 c 7 D þ c 8 D c 4 D c D þ c D c D C ðþ 7 5 Symm c 9 D þ c 0 D ð5þ represents the stiffness change brought about by the damage entities for damage mode. For the special case of laminates with cracks in only 90 plies, we obtain ( ¼ 90 ) C ð90þ pq ¼ t c st 4 a a a 0 5 ðþ symm a wherea i, i ¼,..., 4 are material (laminate) constants to be determined from experimental or computational data on stiffness degradation. It can be observed that the orthotropic symmetry is retained by intralaminar cracking in crossply laminates. In the above relations, ð the constraint parameter ¼ u Þ t c where u and tc represent the COD averaged over the crack surfaces and the thickness of the cracked 90 layer, respectively. The engineering moduli for the cracked laminate can be obtained from the following relationships: E x ¼ C C C C E y ¼ C C C C xy ¼ C C G xy ¼ C Thus, for laminates with 90 ply cracks only, E 0 x E x ¼ 0 þ Da xy 0 yx E 0 y E y ¼ 0 þ Da xy 0 yx xy ¼ 0 xy E0 y 0 þ Da 4 xy 0 yx E 0 y 0 þ Da xy 0 yx G xy ¼ G 0 xy þ Da where " # 0 xy E0 y 0 þ Da 4 xy 0 yx E 0 y 0 þ Da xy 0 yx " # D ¼ t c st 0 xy E0 y 0 þ Da 4 xy 0 yx E 0 x 0 þ Da xy 0 yx ð7þ ð8þ ð9þ As seen from equation (8), the shear modulus is uncoupled from the other three moduli and thus can be treated independently. The four constants appearing in these relations are evaluated by using initial elastic properties and their values at one crack spacing. Thus, if the chosen crack spacing is s 0, then " # a ¼ E x E 0 x D 0 xy yx 0 xy 0 yx " # E 0 y a ¼ E y D 0 xy yx 0 xy 0 yx a ¼ h i G xy G D 0 xy 0 " # a 4 ¼ xy E y 0 xy E0 y D 0 xy yx 0 xy 0 yx with D 0 ¼ D s¼s0 ¼ t c s 0 t. ð0þ Downloaded from jcm.sagepub.com at UNIV TORONTO on January 5, 0
7 Singh and Talreja 7 Case : multiple damage modes. The details of damage modeling in multidirectional laminates with cracking in multiple offaxis plies are given in References [9 ] and reproduced in Appendix A for the sake of completeness. For the special case of [0 m / 90 r / n ] s and [0 m / n /90 r ] s laminates with intralaminar cracks in þ, and 90 layers, the stiffnessdamage relations are same as in equation (8) except that D is now given by 8 D ¼ t 0 t s n ð þ rþ 904nþr r 90 þ r 90 n j ¼90 s 90 ðþ with the following constraint parameters ¼ u 4n ; 904nþr ¼ u 90 4nþr ; 90 ¼ u 90 r 4nt 0 ð4n þ rþt 0 rt 0 ðþ for [0 m /90 r / n ] s laminates, and D ¼ 4t 0 t s n ð þ rþ 904nþr r 90 þ r 90 n j ¼90 s 90 ðþ with the following constraint parameters ¼ u n ; 904nþr ¼ u 90 4nþr ; 90 ¼ u 90 r nt 0 ð4n þ rþt 0 rt 0 ð4þ for [0 m / n /90 r ] s laminates, where t 0 is the thickness of a single ply, s n, and s90 are the normal crack spacings in and 90 plies, respectively. In expressions for the constraint parameters, the subscript denotes a particular damage mode (orientation of cracked plies) and subsubscript represents the number of cracked plies corresponding to that damage mode. The flow chart in Figure describes the procedure for multiscale synergistic methodology for multimode damage assessment taking an example of [0 m / n /90 r ] s laminates. Computational micromechanics involves analysis of a representative unit cell to determine the COD values and the constraint parameters. In a separate step, the material constants a i appearing in equations (8) and (0) are determined from experiments or numerical simulations carried for a reference laminate, specifically [0/90 ] s. These relations are then employed to predict stiffness degradation with constraint parameters and material constants obtained from experiments (or FE simulations) as inputs. In the final step, the overall structural behavior in response to external loading can be analyzed based on the degraded stiffness properties for the damaged laminate. A reference laminate in principle could be any crossply laminate of a chosen configuration. The procedure for predicting crackinginduced property changes for other crossply laminates is independent of this choice. The specific choice of [0/90 ] s laminate was made here as experimental data for this laminate was available from which the constrained parameter could be estimated. The procedure described above for determining elastic moduli changes in a laminate requires calculating CODs of ply cracks. However, the laminate elastic moduli can change additionally due to the nonlinear shear response of plies. In References [8,0] a procedure for correcting the CDM predictions by including this response was illustrated. Modeling of damage evolution For predicting evolution of ply cracking, the authors have developed an energybased approach, which is capable of dealing with cracking in offaxis plies of orthotropic laminates. In Reference [5], the approach is described and applied to several ply cracking cases. Here, we apply it to the relevant WWFEIII test cases. A brief description of the approach follows. As illustrated in Figure 4, two damage states are considered: State with N parallel offaxis cracks spaced at distance s, and State where the cracks have multiplied to N and attained spacing s/. The crack density is assumed to increase when the work required in going from State to State (which is the Figure 4. Progressive multiplication of intralaminar cracks in an offaxis ply. Downloaded from jcm.sagepub.com at UNIV TORONTO on January 5, 0
8 8 Journal of Composite Materials 0(0) same as work needed to close N cracks in going from State to State ) exceeds a critical value, i.e., if in a general offaxis ply, one can use a multimode criterion given as W N!N N:G c sin t c ð5þ M þ w N II ðþ w I G Ic G IIc where is the offaxis angle shown in Figure and G c is the critical (threshold) value of energy required for ply crack formation within the given laminate (more discussion about this later). The work required to form additional N cracks in going from State to State is therefore, W N!N ¼ W N!0 W N!0 ðþ where W N!0 and W N!0 represent work required to close N cracks in State, and N cracks in State, respectively, and the two quantities are calculated as (see Reference [] for detailed derivation) W N!0 ¼ N sin ðt cþ h ð0 E Þ : ~u n ðsþþ i 0 ~u n ðsþ W N!0 ¼ N sin ðt cþ : E ð7þ h ð0 Þ: s ~u n þ 0 ~u s i t ð8þ where ~u n, ~u t are the normalized average crack opening and sliding displacements (COD and CSD). These are given by ~u n ¼ u n t c 0 =E ¼ t c 0 =E ~u t ¼ u t t c 0 =E ¼ t c 0 =E Z t = t c = Z t = t c = u n ðþdz z u t ðþdz z ð9þ where u n and u t represent the relative opening and sliding displacement of the cracked surfaces, respectively, and overbars represent averages. For the special case of cracking in 90 ply only, the sliding displacement is zero (under uniaxial loading condition) and hence the criterion for ply multiplication is written as 0 h t c : ~u s i n ~u n ðsþ G Ic E ð0þ where G Ic is the critical energy release rate in Mode I (crack opening mode). This is the same relation as derived for cracking in crossply laminates by Joffe et al. except that they consider centrally placed cracked 90 plies in their model and normalize the average COD with half the ply thickness (t c /). For cracking where w I ¼ ð 0 Þ E w II ¼ ð 0 Þ t c E h : ~u s i n ~u n ðsþ ; h : ~u s i t ~u t ðsþ ðþ and G IIc is the critical energy release rate in Mode II (crack sliding mode), and the exponents M and N depend on the material system, for example, for glass/ epoxy M ¼, N ¼. 5 In our work, 5 we interpret the critical material parameters G IC and G IIC not in the usual linear elastic fracture mechanics sense where they are defined as the resistance to advancement of the crack front at the point of unstable crack growth. Instead, we postulate that the work required to go from State to State involves a range of dissipative processes that all depend on the material condition in a cracking ply within the given laminate. The material parameter representing the dissipated energy per unit of ply crack surface is, therefore, not what is obtained in a standard fracture toughness test for determining G Ic or G IIc. Furthermore, as discussed in Reference [5], we believe a ply crack cannot form unless sufficient energy is available to open its surfaces (i.e. mode I). In other words, a pure sliding action will not generate a set of parallel cracks illustrated in Figure 4. This will imply that the second term in equation () is negligible. In fact, we report good predictions of crack density evolution by only using the first term in equation (). Also, we do not use the conventional G Ic but extract this value from test data of a reference laminate and use it to make predictions for other laminates. For the WWFEIII, however, we are given conventional G Ic and G IIc and have used those. Thus, the predictions reported here will not be in accordance with our analysis proposed in Reference [5]. Analysis method The prediction of overall stress strain response for a given damaged laminate using CDM entails following steps:. Determine damage constants a i that appear in the damagestiffness relations (equation (8), using equation (0)). This task requires stiffness constants Downloaded from jcm.sagepub.com at UNIV TORONTO on January 5, 0
9 Singh and Talreja 9 for virgin (undamaged) laminate, E 0 x, E0 y, G0 xy, v0 xy, and moduli of cracked laminates at some specified crack spacing, s 0 : E x ðs 0 Þ, E y ðs 0 Þ, G xy ðs 0 Þ, v xy ðs 0 Þ. The moduli for virgin laminate are obtained through the classical laminated plate theory (CLT) by using the properties of a unidirectional lamina, whereas their values at crack spacing s 0 are obtained by micromechanical analysis using finite element method (FEM) for reference laminate [0/90 ] s. In earlier works, e.g., References [8,0], these constants were obtained using experimental data for stiffness changes. It is noted here that the choice of a reference laminate is driven by convenience and availability of experimental data. Since in earlier works 8,0 the [0/90 ] s laminate was used to obtain the material constants, the same laminate was then used in later work as the reference laminate for FEM calculations.. Find stiffness constants as a function of crack density ( c ¼ /s) using equation (8), depending on the laminate type. This gives, C ijkl ¼ f ð c Þ ðþ. Predict evolution of crack density as a function of applied axial strain using the fracture criterion expressed in equation (0). Thus, c ¼ f " ij ð4þ The strain to initiation of first multiple cracking can be estimated by backward extrapolation of the function f. 4. Combine results from steps and (equations () (4)) to obtain stiffness properties as a function of applied strain, equation (5), and predict the overall stress strain response of the laminate for axial tensile loading along laminate longitudinal direction. C ijkl ¼ c ijkl " ij ð5þ Computational micromechanics (FE analysis). As described above, SDM approach requires evaluation of COD and damage constants, experimentally or computationally. Since the BVP for multidirectional laminates is inherently threedimensional, we use D FE analysis to compute these parameters. For the reference crossply laminate, the representative unit cell is as shown in Figure 5. For this laminate layup, periodic boundary conditions are applied to the end faces in the transverse (y) direction, and laminate symmetry about the midplane is achieved by having outofplane displacements (w) zero at the symmetry plane. Uniform displacement is prescribed on the right face of the cell to have tensile loading. However, for multidirectional laminates with cracks in more than two orientations (e.g. multimode cracking in [0/90/þ/] laminates), the construction of FE model is somewhat complex and is detailed in References [,5]. For SDM predictions for laminates, we chose [0/90 ] s, i.e. ¼ 90, as a reference laminate. The stiffness damage results for this crossply laminate can be obtained in a variety of ways. The most obvious way would be by using experimental data. However, although experiments reflect the real material behaviour, they can be performed for limited cases. An alternative and more general way is to use a numerical tool such as an FE model to simulate stiffness degradation. FE simulations are in fact easier to carry out and have no scatter other than the accuracy of computations that may depend on mesh density and implementation of boundary conditions. The crack density along x direction (or equivalently, the crack spacing) was varied by changing the length of the unit cell considered. Linear elastic FE analyses were carried using ANSYS 7 for the reference laminate. The cracks were assumed to be fully grown through thickness and width of 90 plies. The longitudinal modulus and the Poisson s ratio of the damaged laminate were obtained using the volume averaging 8 of stresses and strains as given by Figure 5. Representative unit cell for FE analysis of reference [0/90 ] s laminate. The applied displacement boundary conditions are shown above. Periodic boundary conditions are applied on end faces in the width (y) direction. Downloaded from jcm.sagepub.com at UNIV TORONTO on January 5, 0
10 0 Journal of Composite Materials 0(0) the following equations h E x ¼ xxi h i " xx xy ¼ " yy h i " xx ðþ ð7þ where brackets <> specify volume averaging. CODs averaged over thickness of the cracked ply are calculated from u ¼ t c Z tc= t c = u ðþdz z ð8þ where u ¼ u þ u represents the separation of crack planes in the direction normal to the crack face in the local lamina coordinate system x, x, x with x along crack longitude, x transverse to the crack and x along ply thickness. Numerically, u is determined from nodal x direction displacements averaged over the entire crack surface. The above micromechanical expressions are exact in the sense that they do not involve any homogenization theory and are directly calculated from FE data. Errors in the calculations can be only due to approximation in FE analysis. Further details on FE analysis methodology and validation for multidirectional laminates can be found in References [0,,5,9,0]. It should be pointed out here that we have not included thermal stresses caused by cooling down of the composite laminates to the room temperature. However, it can be easily taken into account during prediction of damage evolution by including thermal stresses, which are calculated here by classical laminate plate theory (CLT). We demonstrate the effect of thermal stresses on one of the test cases: Test case 4. The coefficient of thermal expansion is assumed to be constant during entire loading process. Hence, we neglect any change in thermal expansion brought about by ply cracking. Theoretical prediction of the WWFEIII test cases The SDM model, by itself, is limited to the prediction of effect of subcritical damage (matrix cracking, for the present scenario) on the stiffness properties of the laminated structure. Unlike the lamina failure theories, it cannot predict the lamina or laminate failure. Hence, our analysis here is limited to the test cases where effect of damage on the stress strain response is desired. The test cases, thus analyzed are Test Case, Test Case 4, Test Case, Test Case 7, Test Case 8, Test Case and Test Case. The input data for the analysis performed here is taken from Reference []. In the first step, we carried out FE simulations to characterize stiffness properties for reference laminate [0/90 ] s for all material types. Thickness of a single ply is taken as 0.5 mm. The crack density for these calculations in simulations was taken to be equal to.0 cr/ mm. Axial tensile loading along laminate longitude was applied to the representative unit cell shown in Figure 5. The changes are thus assumed to occur only in E x, and v xy, where as E y and G xy are assumed to be impervious to damage for this laminate layup. The relative stiffness properties, constraint parameters, D 0, and the corresponding damage constants for three material systems, viz. Glass/epoxy (Glass/LY55), G4 800/ 50 and IM7/855 targeted in this study, are shown in Table. These constants were assumed to be the same for different test cases as long as the ply material remains the same. To evaluate the stiffness changes for various test layups, the constraint parameters were obtained in each case for crack density equal to 0. cr/mm (see Tables and for calculated COD values for different test cases). Then using expressions in equation (8), stiffness properties for other laminates were obtained. In doing so, it must be emphasized that since the damage constants are laminatedependent, they must be adjusted in case the thickness of the cracked ply in the laminate configuration changes, e.g., for Test Table. Stiffness properties and constraint parameters for reference [0/90 ] s laminates made for different materials. The relative stiffness changes are determined from FE simulations at crack density equal to cr/mm, whereas the constraint parameters are calculated at an assumed initial crack density equal of 0. cr/mm Material type Constraint parameter, D 0 E x =E 0 x v xy =vxy 0 Damage constants, a i (GPa) a a a a 4 Glass/epoxy (Glass/LY55) 7.e 4.8e G4800/50 5.5e.8e IM7/ e.5e Downloaded from jcm.sagepub.com at UNIV TORONTO on January 5, 0
11 Singh and Talreja Case 4: [0/90 4 ] s laminate, a 0 ¼ a ðc 0 Þ ½0=90 4 Š s ; a ½0=90 0 ¼ a ðc 0 Þ ½0=90 4 Š s ; Š s ½0=90 Š s C 0 C 0 a 0 ¼ a ðc 0 Þ ½0=90 4 Š s ; a ½0= ¼ a ðc 0 Þ ½0=90 4 Š 4 s ð9þ Š s ½0=90 Š s C 0 C 0 where ai 0 represents reevaluated constants for the laminate in consideration and a i represents constants for the reference laminate. Thus, the constants a i s are recalculated every time the relative thickness of layers in the laminate changes. To simulate the stress strain response, we need damage evolution predictions. For this purpose, an Table. Calculated average COD values for 90 cracking for selected test cases. All COD values are in mm Crack density (/mm) Test Case Test Case 4 Test Case Test Case 7 Test Case COD: crack opening displacement. Table. Calculated average COD values for 90 cracking for Test Cases and. All COD values are in mm Crack density (/mm) Test Case Test Case, m ¼ Test Case, m ¼ Test Case, m ¼ COD: crack opening displacement. Downloaded from jcm.sagepub.com at UNIV TORONTO on January 5, 0
12 Journal of Composite Materials 0(0) Figure. Stiffness and Poisson s ratio degradation for Test Case : [0/90/0] T glass/epoxy laminate. Figure 7. Stress strain response and crack density evolution for Test Case : [0/90/0] T glass/epoxy laminate. No thermal effects were taken into account. energybased fracture criterion given in equation (0) was utilized in a MATLAB code. The normalized average COD and CSD for different crack spacing were obtained using FE simulations on the representative unit cell for the respective laminate. For 90 cracking, the calculated COD values are tabulated in Table (CSD ¼ 0 for 90 cracks). Polynomial fits to these COD values were used in the simulation for damage evolution. The damage evolution subroutine was run until the applied strain reaches longitudinal failure strain in tension. If the calculated crack initiation strain comes out to be higher than the longitudinal failure strain, the laminate is understood to have failed by fibre fractures. Downloaded from jcm.sagepub.com at UNIV TORONTO on January 5, 0
13 Singh and Talreja Figure 8. Stiffness and Poisson s ratio degradation for Test Case 4 [0/90 8 /0] T glass/epoxy laminate. For stiffness changes, the damage model considered in the present study is a linear model with respect to the crack density. A nonlinear model will involve additional damage constants and would be required to achieve a better accuracy for high crack density. For present purpose of illustration, a linear approach is sufficient. Test Case. For this test case, Figure shows the variation of longitudinal Young s modulus and the Poisson s ratio normalized with initial values E x, xy E 0 x 0 xy against the normalized crack density ( 90 t 90 ). The evolution of crack density and corresponding stress strain response are shown in Figure 7. For this laminate case, the ply cracks initiate in 90 plies at an applied axial strain of about.%. After initiation, cracks grow in number very quickly on increase in applied strain and reach a saturation level subsequently. The overall shape of crack density increase is parabolic. The value of 90 t 90 reached at longitudinal tensile failure strain (" T ¼ :807%) for this material is slightly more than.0, suggesting a very high value of absolute crack density (8 cracks/mm). Still the effect on stress strain response is not too severe as would be for thicker 90 plies (such as in the next Test Case). Although the Poisson s ratio reduces, its effect on the transverse stress strain curve ( x vs. " y ) is almost negligible. Test Case 4. For this test case, the laminate material is same as in the previous one. However, the thickness of the 90 plies is eight times of that in the previous case. Consequently, the degradation in the laminate stiffness due to ply cracking is much more severe in the present case (see Figure 8). Also, the ply cracks in 90 plies initiate at much lower applied strain of about 0.7%. As compared to the Test Case, however, the rate of damage evolution is lower in this case and the value of 90 t 90 reached at " x ¼ " T for this material is 0., suggesting much lower absolute crack density (0. cracks/ mm). The shape of the damage evolution curve is quite similar to that in Test Case (Figure 9). The stress strain response (also in Figure 9) is significantly nonlinear after ply cracking. For thicker cracked plies, thus, ply cracking may cause severe nonlinearity in the longitudinal stress strain response. Although there is large reduction in the Poisson s ratio subsequent to ply cracking, its effect on the transverse stress strain curve ( x vs:" y ) is not visible. Here, we also illustrate the effect of thermal residual stresses on ply cracking and the resultant stress strain response. Due to differential thermal expansion of longitudinal and transverse plies, the inner 90 ply will develop compressive thermal residual strains when it is cooled from curing to the room temperature. The residual thermal strains due to thermal effects during curing are calculated using CLT as " th t 0 E ¼ t 0 E þ t 90 E T 45: ¼ :4 8: 4 : þ 45: ð Þ0 ð0 5Þ ¼ : :07% ð40þ where t 0 is 0 ply thickness, and T ¼ T ref T service with T service ¼ 5 C being the service (room) Downloaded from jcm.sagepub.com at UNIV TORONTO on January 5, 0
14 4 Journal of Composite Materials 0(0) Figure 9. Stress strain response and crack density evolution for Test Case 4: [0/90 8 /0] T glass/epoxy laminate. Dashed lines (denoted in legend by second subscript t) include the effect of strains generated due to thermal mismatch between 0 and 90 plies during curing on damage initiation and progression. temperature, T ref ¼ 0 C being the curing (stress free) temperature. The crack initiation strain thus decreases by 0.07% from the earlier value obtained without considering thermal effects. The rate of damage progression is however independent of thermal residual stresses. Thus, the new damage evolution curve just gets shifted to the left of the curve without such effects by an amount equal to thermal residual strain. The stress strain response is also affected as shown in Figure 9 by dashed lines (using second subscript t in legend). Thermal effects are observed to be small for transverse stress strain response. Test Case. For multidirectional laminates, the damage will form in multiple plies of different orientations. For the specific case of quasiisotropic laminates considered here in Test Cases 8, the cracks may form in 90, þ45 and 45 layers. The combined effect of these cracks is felt more severely on the overall stiffness properties. Although most of stiffness degradation comes from 90 cracks, 45 cracks may interact with 90 cracks and cause more severe degradation than what would be observed if cracks in these different damage modes occurred without affecting each other. SDM model is capable of dealing with this multimode damage scenario, as depicted by stiffnessdamage relationships with D described in equations () (4). Obviously, the density and opening displacements of intralaminar cracks in a given layer will depend on the material, orientation and the thickness of that ply and also on the relative constraint on the cracked ply from surrounding supporting plies. For oblique cracks, sliding of the cracked surfaces will also play a role in the cracking criterion according to equation (). It is often observed in experiments, for example Reference [0], that 45 cracks may not grow fully before the laminate fails by delamination, and therefore we will assume 45 cracks are halfdeveloped, i.e. while evaluating stiffness properties we will reduce the total crack density 45 such that the effective crack density in these plies is given by ð 45 Þ eff ¼ r 45 ; r ¼ 0:5. More detailed information about the growth of cracks is necessary to model this behaviour. This relative density is chosen for illustration purpose only and is based on our experience with model s usage to predict stiffness degradation in quasiisotropic laminates for experimental data on quasiisotropic laminates reported in Reference []. The respective crack densities in different cracked plies are obtained using the damage progression model. Actual experimental observations may be necessary to simulate real material behaviour more accurately. The resulting plots for longitudinal Young s modulus and Poisson s ratio for Test Cases, predicted using expressions in equations (8) and (), are shown in Figure 0. The constraint parameters for 45 cracking with respect to that for 90 cracking are calculated using the parametric equation developed for COD variation with respect to ply orientation in Reference [0] Downloaded from jcm.sagepub.com at UNIV TORONTO on January 5, 0
15 Singh and Talreja 5 Figure 0. Variation of longitudinal Young s modulus and Poisson s ratio: (a) vs. normalized crack density in 90 ply and (b) vs. applied strain for Test Case : [0/90/ 45/þ45] s glass/epoxy laminate. Cracks in all offaxis modes are accounted depending on their respective initiation strains and variation of crack densities with applied strain as shown in the next figure. No thermal effects were taken into account. considering cracking in cracking in [0//0 / ] s Glass/epoxy laminates: u ¼ u 90 sin ð4þ Also, it is assumed that 904nþr ¼ 90 and j ¼90 ¼ 90. It is noted that the above equation may not be accurate when cracks in multiple offaxis orientations are present with different crack densities. A more detailed FE computation with experimentally observed crack densities is warranted in such a case. The COD variation in 45 plies is assumed following equation (4). As a simplification, the cracking in both 45 plies is assumed to initiate at identical applied strain and progress with same rate, although experiments may suggest that the 45 ply that is adjacent to 90 ply may fail earlier. In Figure 0, we first show the variation of laminate stiffnesses with respect to crack density in 90 ply. Because at higher applied strains cracks are present in all offaxis orientations, Figure 0(b) is more appropriate, which shows their variation with respect to the applied strain. The damage progression in all offaxis plies is shown in Downloaded from jcm.sagepub.com at UNIV TORONTO on January 5, 0
16 Journal of Composite Materials 0(0) Figure. Stress strain response and crack density evolution for Test Case : [0/90/ 45/þ45] s glass/epoxy laminate with cracks in all offaxis modes. The crack initiation and the crack density evolution in both 45 plies are assumed to be identical. No thermal effects were taken into account. Figure. Stiffness and Poisson s ratio degradation for Test Case 7: [0/ 45/þ45/90] s G4 800/500 laminate. Figure. The cracks initiate in 90 ply at about 0.% axial strain, and in 45 plies at about.5% axial strain. Initial stiffness degradation (" x 4 0:%) occurs due to 90 cracks only, whereas later (" x 4 :5%) 45 cracks also contribute to stiffness degradation. The evolution curves for normalized crack densities in 95 and 45 plies have similar shapes, with saturation levels of 90 t 90 0:7; 45 t 45 0:. No thermal effects were considered while predicting damage progression and resultant stiffness properties. As a result of ply cracking in multiple orientations, the stiffness degradation is more severe than would be for cracking in 90 plies only. As reported in Reference [], cracks in 45 plies will typically form from 45/90 interfaces and tend to further enhance opening of cracks present in 90 plies. This increases the rate of Downloaded from jcm.sagepub.com at UNIV TORONTO on January 5, 0
17 Singh and Talreja 7 Figure. Stress strain response and crack density evolution for Test Case 7: [0/ 45/þ45/90] s G4 800/500 laminate with cracks in 90 plies only. Strains generated due to thermal mismatch between 45  and 90 plies during curing were taken into account while evaluating damage initiation and progression. damage evolution as well as corresponding degradation in stiffness properties and is not accounted for here. Some nonlinearity is observed in longitudinal and transverse stress strain curves (Figure ). Test Case 7. For this ply material, we observed that our FE calculations on reference laminate [0/90 ] s showed very small relative degradation in E x but significant degradation in v xy (see Table ). The COD, hence the constraint parameter, was also calculated to be smaller with this material. Therefore, the changes in longitudinal Young s modulus are less pronounced for laminate with this material than Glass/epoxy. Figure shows the predicted changes in stiffness properties for this case. The corresponding stress strain response along with crack density evolution is shown in Figure. For laminates made from G4800/50 material, thermal residual stresses generated during curing were found to affect the damage initiation behaviour significantly. For the present layup [0/45/þ45/90] s, the mismatch in axial thermal strains between the 45 and the 90 plies during curing is calculated as 0.%. This decreases the crack initiation strain in 90 plies to about 0.9% (Figure ). The model does not predict any cracking in 45 plies. The shape of crack density evolution is about the same as before with maximum normalized crack density in 90 plies at about 0. at " x ¼ " T. Appreciable nonlinearity is seen in stress strain responses, especially the transverse stress strain response. Test Case 8. When only mechanical strains were considered, our model did not predict any cracking for this laminate (i.e. crack initiation strain for this case was determined to be greater than the provided failure strain for unidirectional lamina). However, when we include residual thermal strains, the cracking in 90  plies is predicted. The reduction in the longitudinal stiffness and Poisson s ratio is predicted to be similar to Test Case 7 (Figure 4) when absolute crack densities are considered. However, the crack initiation and progression behaviour (Figure 5) is quite different mainly due to different thicknesses of 90 plies in the two test cases. For the present case, the mismatch between 0 and 90 plies is important, which is calculated as 0.%. This decreases the crack initiation strain to about.% in 90 plies. Cracks do not form in 45  plies. The normalized crack density is found to rise quickly and the maximum normalized crack density at " x ¼ " T is predicted to be about 0.5, much smaller than that in the Test Case 7. Some nonlinearity in stress strain responses due to cracking is observed. Test Case and. Although these test cases are meant for compressive and tensile strength of the quasiisotropic laminates in the presence of hole, we do not attempt full analysis and prediction here since that would require detailed structural stress analysis. However, we illustrate how SDM model could be applied to laminate cases where ply thickness varies. For given ply layup [45 m /90 m /45 m /0 m ] s in Test Case, we vary m Downloaded from jcm.sagepub.com at UNIV TORONTO on January 5, 0
18 8 Journal of Composite Materials 0(0) Figure 4. Stiffness and Poisson s ratio degradation for Test Case 8: [45/0/90/45] s G4 800/500 laminate. Figure 5. Stress strain response and crack density evolution for Test Case 8: [45/0/90/45] s G4 800/500 laminate with cracks in 90 plies only. Strains generated due to thermal mismatch between 0  and 90 plies during curing were taken into account while evaluating damage initiation and progression. from to 4 with m ¼ 4 equivalent to the Test Case. Cracking in only 90 plies is assumed and the analysis neglects any damage in the 45 and 0 plies. If there is significant cracking in 45 plies, the COD calculations (FE model) as well as stiffness predictions must account for cracks in these offaxis plies also, as was illustrated before in case of Test Case 7. Since the ply sequence and relative thickness of cracked and constrained plies remains the same, the relative stiffness change will be given by the ratio of constraint parameters, i.e. ¼ = 0, where 0 is the constraint parameter obtained for the reference laminate [0/90 ] s. is calculated to be 0.555,0.55, and , respectively, for m ¼ to 4. Thus, the stiffness degradation should be the same in all laminates because their relative thickness is the same; the slight difference may be due to different mesh densities and inaccuracies in COD calculations. The ratio of Downloaded from jcm.sagepub.com at UNIV TORONTO on January 5, 0
19 Singh and Talreja 9 Figure. Stiffness and Poisson s ratio degradation for Test Case : [45/90/45/0] s IM7/855 laminate. For Test Case, [45 m / 90 m / 45 m /0 m ] s laminate, with different m values, the stiffness reduction is about the same because relative thickness of cracked and constraining plies remains constant. Cracking only in 90 plies is assumed. Figure 7. Stress strain response and crack density evolution for Test Case : [45/90/45/0] s IM7/855 laminate with cracks in 90 plies only. No thermal effects were taken into account. degraded to original longitudinal modulus and Poisson s ratio for m ¼ 4 (Test Case ) is shown in Figure. However, the change in thickness has a significant effect on crack initiation and progression. The crack initiation strain decreases as the cracked ply thickness increases. The rate of damage progression is higher for lower m. For a ply thickness of 0.5 mm (m ¼ ), crack initiation strain was calculated to be.79%, which is greater than the longitudinal tensile failure strain (" T ¼.55%) for the UD lamina with this material. Thus, for this value of m and the provided G Ic value, our model predicts no ply cracking before Downloaded from jcm.sagepub.com at UNIV TORONTO on January 5, 0
ISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationTHE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH
THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More information3D and Planar Constitutive Relations
3D and Planar Constitutive Relations A School on Mechanics of Fibre Reinforced Polymer Composites Knowledge Incubation for TEQIP Indian Institute of Technology Kanpur PM Mohite Department of Aerospace
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationFracture Mechanics of Composites with Residual Thermal Stresses
J. A. Nairn Material Science & Engineering, University of Utah, Salt Lake City, Utah 84 Fracture Mechanics of Composites with Residual Thermal Stresses The problem of calculating the energy release rate
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of aterials Science and Engineering A 6 (12) (2016) 3542 doi: 10.17265/21616213/2016.12.005 D DAVID PUBLISHIG Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K
More informationME 582 Advanced Materials Science. Chapter 2 Macromechanical Analysis of a Lamina (Part 2)
ME 582 Advanced Materials Science Chapter 2 Macromechanical Analysis of a Lamina (Part 2) Laboratory for Composite Materials Research Department of Mechanical Engineering University of South Alabama, Mobile,
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationFINITE ELEMENT ANALYSIS OF A LAYERED COMPOSITE CYLINDER USING THE CONNECTION BETWEEN THE MACRO AND MICROSTRUCTURE
FINITE ELEMENT ANALYI OF A LAYERED COMPOITE CYLINDER UING THE CONNECTION BETWEEN THE MACRO AND MICROTRUCTURE A. zekrényes Research Assistant, Department of Applied Mechanics, Budapest University of Technology
More informationUniversity of Bristol  Explore Bristol Research. Early version, also known as preprint
Hallett, S. R., & Wisnom, M. R. (2006). Numerical investigation of progressive damage and the effect of layup in notched tensile tests. Journal of Composite Materials, 40 (14), 12291245. DOI: 10.1177/0021998305057432
More informationMechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA What programs are in PROMAL? Master Menu The master menu screen with five separate applications from
More informationAPPLICATION OF A SCALAR STRAINBASED DAMAGE ONSET THEORY TO THE FAILURE OF A COMPLEX COMPOSITE SPECIMEN
28 TH INTERNATIONAL CONGRESS OF THE AERONAUTICAL SCIENCES APPLICATION OF A SCALAR STRAINBASED DAMAGE ONSET THEORY TO THE FAILURE OF A COMPLEX COMPOSITE SPECIMEN Tuyen Tran*, Dan Simkins**, Shen Hin Lim*,
More informationDESIGN OF COMPOSITE LAMINATED STRUCTURES BY POLAR METHOD AND TOPOLOGY OPTIMISATION
DESIGN OF COMPOSIE LAMINAED SUCUES BY POLA MEOD AND OPOLOGY OPIMISAION A. Jibawy,,3, C. Julien,,3, B. Desmorat,,4, (*), A. Vincenti UPMC Univ Paris 6, UM 79, Institut Jean Le ond d Alembert B.P. 6 4, place
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationEXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 EXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES Esben Lindgaard 1 and Brian
More information*Corresponding author: Keywords: Finiteelement analysis; Multiscale modelling; Onset theory; Dilatational strain invariant.
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MICROMECHANICAL MODELLING OF TEST SPECIMENS FOR ONSET OF DILATATIONAL DAMAGE OF POLYMER MATRIX IN COMPOSITE MATERIALS T. D. Tran 1, D. Kelly 1*, G.
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 16 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationMESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP Wanil Byun*, Seung Jo Kim*, Joris Wismans** *Seoul National University, Republic
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More informationNigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37
Nigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37 APPLICATION OF THE REISSNERS PLATE THEORY IN THE DELAMINATION ANALYSIS OF A THREEDIMENSIONAL, TIME DEPENDENT, NONLINEAR, UNIDIRECTIONAL
More information3D Finite Element analysis of stud anchors with large head and embedment depth
3D Finite Element analysis of stud anchors with large head and embedment depth G. Periškić, J. Ožbolt & R. Eligehausen Institute for Construction Materials, University of Stuttgart, Stuttgart, Germany
More informationMATERIAL MECHANICS, SE2126 COMPUTER LAB 4 MICRO MECHANICS. E E v E E E E E v E E + + = m f f. f f
MATRIAL MCHANICS, S226 COMPUTR LAB 4 MICRO MCHANICS 2 2 2 f m f f m T m f m f f m v v + + = + PART A SPHRICAL PARTICL INCLUSION Consider a solid granular material, a so called particle composite, shown
More informationMicromeso draping modelling of noncrimp fabrics
Micromeso draping modelling of noncrimp fabrics Oleksandr Vorobiov 1, Dr. Th. Bischoff 1, Dr. A. Tulke 1 1 FTA Forschungsgesellschaft für Textiltechnik mbh 1 Introduction Noncrimp fabrics (NCFs) are
More informationInterlaminar fracture characterization in composite materials by using acoustic emission
5th International Symposium on NDT in Aerospace, 1315th November 2013, Singapore Interlaminar fracture characterization in composite materials by using acoustic emission Ian SILVERSIDES 1, Ahmed MASLOUHI
More informationVALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 )
VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials
More informationADVANCES IN THE PROGRESSIVE DAMAGE ANALYSIS OF COMPOSITES
NAFEMS WORLD CONGRESS 13, SALZBURG, AUSTRIA ADVANCES IN THE PROGRESSIVE DAMAGE ANALYSIS OF M. Bruyneel, J.P. Delsemme, P. Jetteur (LMS Samtech, Belgium); A.C. Goupil (ISMANS, France). Dr. Ir. M. Bruyneel,
More informationS. Srinivasan, Technip Offshore, Inc., Houston, TX
9 th ASCE Specialty Conerence on Probabilistic Mechanics and Structural Reliability PROBABILISTIC FAILURE PREDICTION OF FILAMENTWOUND GLASSFIBER Abstract REINFORCED COMPOSITE TUBES UNDER BIAXIAL LOADING
More informationREPRESENTING MATRIX CRACKS THROUGH DECOMPOSITION OF THE DEFORMATION GRADIENT TENSOR IN CONTINUUM DAMAGE MECHANICS METHODS
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 REPRESENTING MATRIX CRACKS THROUGH DECOMPOSITION OF THE DEFORMATION GRADIENT TENSOR IN CONTINUUM DAMAGE MECHANICS METHODS
More informationMultiple SpatioTemporal Scale Modeling of Composites Subjected to Cyclic Loading
Multiple SpatioTemporal Scale Modeling of Composites Subjected to Cyclic Loading Robert Crouch 1, Caglar Oskay 1, and Stephen Clay 2 1 Department of Civil and Environmental Engineering, Vanderbilt University,
More informationModule 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More informationCHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles
CHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles Mark Hughes 14 th March 2017 Today s learning outcomes To understand the role of reinforcement, matrix and
More informationEFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING
Journal of MECHANICAL ENGINEERING Strojnícky časopis, VOL 67 (217), NO 1, 522 EFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING Arnab Choudhury 1,
More informationGeneric Strategies to Implement Material Grading in Finite Element Methods for Isotropic and Anisotropic Materials
University of Nebraska  Lincoln DigitalCommons@University of Nebraska  Lincoln Engineering Mechanics Dissertations & Theses Mechanical & Materials Engineering, Department of Winter 1292011 Generic
More informationDon Robbins, Andrew Morrison, Rick Dalgarno Autodesk, Inc., Laramie, Wyoming. Abstract
PROGRESSIVE FAILURE SIMULATION OF ASMANUFACTURED SHORT FIBER FILLED INJECTION MOLDED PARTS: VALIDATION FOR COMPLEX GEOMETRIES AND COMBINED LOAD CONDITIONS Don Robbins, Andrew Morrison, Rick Dalgarno Autodesk,
More informationPRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses
OPTIMAT BLADES Page 1 of 24 PRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses first issue Peter Joosse CHANGE RECORD Issue/revision date pages Summary of changes draft 241002
More information6. NONLINEAR PSEUDOSTATIC ANALYSIS OF ADOBE WALLS
6. NONLINEAR PSEUDOSTATIC ANALYSIS OF ADOBE WALLS Blondet et al. [25] carried out a cyclic test on an adobe wall to reproduce its seismic response and damage pattern under inplane loads. The displacement
More informationUnderstand basic stressstrain response of engineering materials.
Module 3 Constitutive quations Learning Objectives Understand basic stressstrain response of engineering materials. Quantify the linear elastic stressstrain response in terms of tensorial quantities
More informationIMPACT ON LAMINATED COMPOSITE PLATES: COMPARISON OF TEST AND SIMULATION RESULTS OBTAINED WITH LMS SAMTECH SAMCEF
V ECCOMAS Thematic Conference on the Mechanical Response of Composites COMPOSITES 015 S.R. Hallett and J.J.C. Remmers (Editors) IMPACT ON LAMINATED COMPOSITE PLATES: COMPARISON OF TEST AND SIMULATION RESULTS
More informationMalaysia Phone: ; Fax:
International Conference on Mechanical Engineering Research (ICMER013), 13 July 013 Bukit Gambang Resort City, Kuantan, Pahang, Malaysia Organized By Faculty of Mechanical Engineering, Universiti Malaysia
More informationSUBSURFACE DAMAGE LOCATION AND IDENTIFICATION USING INFRARED TECHNIQUES
SUBSURFACE DAMAGE LOCATION AND IDENTIFICATION USING INFRARED TECHNIQUES T.R. Emery 1, J. M. DulieuBarton 1, P.R. Cunningham 2 1 University of Southampton, School of Engineering Sciences, SO17 1BJ, UK
More informationSize Effects In the Crushing of Honeycomb Structures
45th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics & Materials Conference 1922 April 2004, Palm Springs, California AIAA 20041640 Size Effects In the Crushing of Honeycomb Structures Erik C.
More informationMechanical properties 1 Elastic behaviour of materials
MME131: Lecture 13 Mechanical properties 1 Elastic behaviour of materials A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Today s Topics Deformation of material under the action of a mechanical
More informationFASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS FASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES G. Catalanotti 1*, P.P. Camanho 1, P. Ghys 2, A.T. Marques 1 1 DEMec, Faculdade de Engenharia, Universidade
More informationCHARACTERIZATION, ANALYSIS AND PREDICTION OF DELAMINATION IN COMPOSITES USING FRACTURE MECHANICS
Oral Reference Number: ICF100942OR CHARACTERIZATION, ANALYSIS AND PREDICTION OF DELAMINATION IN COMPOSITES USING FRACTURE MECHANICS T. Kevin O Brien U.S. Army Research Laboratory Vehicle Technology Directorate
More informationEffects of geometry and properties of fibre and matrix on overall. composite parameters
Int. Journal of Applied Sciences and ngineering Research, ol. 3, Issue 4, 2014 www.ijaser.com 2014 by the authors Licensee IJASR Under Creative Commons License 3.0 editorial@ijaser.com Research article
More informationUSING A HOMOGENIZATION PROCEDURE FOR PREDICTION OF MATERIAL PROPERTIES AND THE IMPACT RESPONSE OF UNIDIRECTIONAL COMPOSITE
Volume II: Fatigue, Fracture and Ceramic Matrix Composites USING A HOMOGENIZATION PROCEDURE FOR PREDICTION OF MATERIAL PROPERTIES AND THE IMPACT RESPONSE OF UNIDIRECTIONAL COMPOSITE A. D. Resnyansky and
More informationA FINITE ELEMENT MODEL FOR THE ANALYSIS OF DELAMINATIONS IN FRP SHELLS
TRENDS IN COMPUTATIONAL STRUCTURAL MECHANICS W.A. Wall, K.U. Bletzinger and K. Schweizerhof (Eds.) c CIMNE, Barcelona, Spain 2001 A FINITE ELEMENT MODEL FOR THE ANALYSIS OF DELAMINATIONS IN FRP SHELLS
More informationEFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES
EFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES OF WOOD OR PLYWOOD CONSIDERED AS ORTHOTROPIC MATERIALS Information Revied and Reaffirmed March 1956 No. 1510 EFFECT OF ELLIPTIC
More informationScienceDirect. Unit cell model of woven fabric textile composite for multiscale analysis. Anurag Dixit a *,Harlal Singh Mali b, R.K.
Available online at www.sciencedirect.com ScienceDirect Procedia Engineering 68 ( 2013 ) 352 358 The Malaysian International Tribology Conference 2013 (MITC2013) Unit cell model of woven fabric textile
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationAn investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading
An investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading A. Makris, C. Ramault, D. Van Hemelrijck Department of Mechanics of Materials and Constructions,
More informationAnisotropic modeling of short fibers reinforced thermoplastics materials with LSDYNA
Anisotropic modeling of short fibers reinforced thermoplastics materials with LSDYNA Alexandre Hatt 1 1 Faurecia Automotive Seating, Simplified Limited Liability Company 1 Abstract / Summary Polymer thermoplastics
More informationChapter 6: Mechanical Properties of Metals. Dr. Feras Fraige
Chapter 6: Mechanical Properties of Metals Dr. Feras Fraige Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility Toughness
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 15 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationConstitutive models: Incremental (Hypoelastic) Stress Strain relations. and
Constitutive models: Incremental (Hypoelastic) Stress Strain relations Example 5: an incremental relation based on hyperelasticity strain energy density function and 14.11.2007 1 Constitutive models:
More informationEnergy release rate analysis for adhesive and laminate double cantilever beam specimens emphasizing the effect of residual stresses
International Journal of Adhesion & Adhesives 20 (1999) 59 70 International Journal of Adhesion & Adhesives Energy release rate analysis for adhesive and laminate double cantilever beam specimens emphasizing
More informationComposite Laminate Modeling
omposite Laminate Modeling White Paper for Femap and NX Nastran Users Venkata Bheemreddy, Ph.D., Senior Staff Mechanical Engineer Adrian Jensen, PE, Senior Staff Mechanical Engineer WHAT THIS WHITE PAPER
More information14. LSDYNA Forum 2016
14. LSDYNA Forum 2016 A Novel Approach to Model Laminated Glass R. Böhm, A. Haufe, A. Erhart DYNAmore GmbH Stuttgart 1 Content Introduction and Motivation Common approach to model laminated glass New
More informationPractical methodology for inclusion of uplift and pore pressures in analysis of concrete dams
Practical methodology for inclusion of uplift and pore pressures in analysis of concrete dams Michael McKay 1 and Francisco Lopez 2 1 Dams Engineer, GHD Pty 2 Principal Dams/Structural Engineer, GHD Pty
More informationLAMINATED COMPOSITE PLATES
LAMINATED COMPOSITE PLATES David Roylance Department of Materials Science and Engineering Massachusetts Institute of Technology Cambridge, MA 02139 February 10, 2000 Introduction This document is intended
More informationComposite Materials 261 and 262
Composite Materials 261 and 262 Stefan Hartmann 1 David Moncayo 2 1 DYNAmore GmbH, Stuttgart, Germany 2 Daimler AG, Sindelfingen, Germany 11. LSDYNA Forum 2012, 9.  10. Oktober 2012, Ulm 1 Outline Introduction
More informationContinuum Mechanics. Continuum Mechanics and Constitutive Equations
Continuum Mechanics Continuum Mechanics and Constitutive Equations Continuum mechanics pertains to the description of mechanical behavior of materials under the assumption that the material is a uniform
More informationSOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
Mechanical Testing and Diagnosis ISSN 2247 9635, 2012 (II), Volume 3, 7985 SOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Valeriu DULGHERU, Viorel BOSTAN, Marin GUŢU Technical University
More information2D damping predictions of fiber composite plates: Layup effects
Available online at www.sciencedirect.com Composites Science and Technology 68 (2008) 727 733 COMPOSITES SCIENCE AND TECHNOLOGY www.elsevier.com/locate/compscitech 2D damping predictions of fiber composite
More informationFINITE ELEMENT MODELING OF DELAMINATION DAMAGE IN CARBON FIBER LAMINATES SUBJECT TO LOWVELOCITY IMPACT AND
FINITE ELEMENT MODELING OF DELAMINATION DAMAGE IN CARBON FIBER LAMINATES SUBJECT TO LOWVELOCITY IMPACT AND COMPARISON WITH EXPERIMENTAL IMPACT TESTS USING NONDESTRUCTIVE VIBROTHERMOGRAPHY EVALUATION A
More informationCOMPUTER AIDED DESIGN IN CASE OF THE LAMINATED COMPOSITE MATERIALS
6 th International Conference Computational Mechanics and Virtual Engineering COMEC 15 1516 October 15, Braşov, Romania COMPUER AIDED DESIGN IN CASE OF HE LAMINAED COMPOSIE MAERIALS Camelia Cerbu ransilvania
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationNumerical simulation of delamination onset and growth in laminated composites
Numerical simulation of delamination onset and growth in laminated composites G. Wimmer, C. Schuecker, H.E. Pettermann Austrian Aeronautics Research (AAR) / Network for Materials and Engineering at the
More informationTHREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT
THREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT Víctor Martínez 1, Alfredo Güemes 2, Norbert Blanco 1, Josep Costa 1 1 Escola Politècnica Superior. Universitat de Girona. Girona, Spain (17071) 2
More informationEVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS EVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS T. Kurashiki 1 *, Y. Matsushima 1, Y. Nakayasu
More informationUSE OF FINITE ELEMENT METHOD TO EVALUATE THE STRENGTH RESPONSE OF NOTCHED COMPOSITE LAMINATES UNDER TENSION ARJUN KOTHIDAR
USE OF FINITE ELEMENT METHOD TO EVALUATE THE STRENGTH RESPONSE OF NOTCHED COMPOSITE LAMINATES UNDER TENSION By ARJUN KOTHIDAR A thesis submitted in partial fulfillment of the requirements for the degree
More informationChapter 2  Macromechanical Analysis of a Lamina. Exercise Set. 2.1 The number of independent elastic constants in three dimensions are: 2.
Chapter  Macromechanical Analysis of a Lamina Exercise Set. The number of independent elastic constants in three dimensions are: Anisotropic Monoclinic 3 Orthotropic 9 Transversely Orthotropic 5 Isotropic.
More informationNumerical investigation on the position of holes for reducing stress concentration in composite plates with bolted and riveted joints
THEORETICAL & APPLIED MECHANICS LETTERS 1, 041005 (2011) Numerical investigation on the position of holes for reducing stress concentration in composite plates with bolted and riveted joints M. R. Khoshravan,
More informationID1160 REALTIME DETECTION AND EXPLICIT FINITE ELEMENT SIMULATION OF DELAMINATION IN COMPOSITE LAMINATES UNDER IMPACT LOADING
ID116 REALTIME DETECTION AND EXPLICIT FINITE ELEMENT SIMULATION OF DELAMINATION IN COMPOSITE LAMINATES UNDER IMPACT LOADING K. Minnaar and M. Zhou = School of Mechanical Engineering Georgia Institute
More informationFRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING.
FRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING. X. J. Gong, F. Hernandez, G. Verchery. ISAT  Institut Supérieur de l Automobile et des Transports, LRMA  Laboratoire de
More informationCellular solid structures with unbounded thermal expansion. Roderic Lakes. Journal of Materials Science Letters, 15, (1996).
1 Cellular solid structures with unbounded thermal expansion Roderic Lakes Journal of Materials Science Letters, 15, 475477 (1996). Abstract Material microstructures are presented which can exhibit coefficients
More informationStress, Strain, Mohr s Circle
Stress, Strain, Mohr s Circle The fundamental quantities in solid mechanics are stresses and strains. In accordance with the continuum mechanics assumption, the molecular structure of materials is neglected
More informationA MULTISCALE MODELING APPROACH FOR THE PROGRESSIVE FAILURE ANALYSIS OF TEXTILE COMPOSITES MAO JIAZHEN NATIONAL UNIVERSITY OF SINGAPORE
A MULTISCALE MODELING APPROACH FOR THE PROGRESSIVE FAILURE ANALYSIS OF TEXTILE COMPOSITES MAO JIAZHEN NATIONAL UNIVERSITY OF SINGAPORE 2014 A MULTISCALE MODELING APPROACH FOR THE PROGRESSIVE FAILURE ANALYSIS
More informationContinuum mechanics V. Constitutive equations. 1. Constitutive equation: definition and basic axioms
Continuum mechanics office Math 0.107 ales.janka@unifr.ch http://perso.unifr.ch/ales.janka/mechanics Mars 16, 2011, Université de Fribourg 1. Constitutive equation: definition and basic axioms Constitutive
More informationTransactions on Engineering Sciences vol 13, 1996 WIT Press, ISSN
Computational debonding analysis of a thermally stressed fiber/matrix composite cylinder F.G. Buchholz," O. Koca* "Institute ofapplied Mechanics, University ofpaderborn, D33098 Paderborn, Germany ^Institute
More informationReference material Reference books: Y.C. Fung, "Foundations of Solid Mechanics", Prentice Hall R. Hill, "The mathematical theory of plasticity",
Reference material Reference books: Y.C. Fung, "Foundations of Solid Mechanics", Prentice Hall R. Hill, "The mathematical theory of plasticity", Oxford University Press, Oxford. J. Lubliner, "Plasticity
More informationPLAT DAN CANGKANG (TKS 4219)
PLAT DAN CANGKANG (TKS 4219) SESI I: PLATES Dr.Eng. Achfas Zacoeb Dept. of Civil Engineering Brawijaya University INTRODUCTION Plates are straight, plane, twodimensional structural components of which
More informationComparison of Asbuilt FEA Simulations and Experimental Results for Additively Manufactured Dogbone Geometries.
Clemson University TigerPrints All Theses Theses 52017 Comparison of Asbuilt FEA Simulations and Experimental Results for Additively Manufactured Dogbone Geometries. Prathamesh Baikerikar Clemson University,
More informationCalculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites
Copyright c 2007 ICCES ICCES, vol.1, no.2, pp.6167, 2007 Calculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites K. Gordnian 1, H. Hadavinia 1, G. Simpson 1 and A.
More informationModeling Hailstone Impact onto Composite Material Panel Under a Multiaxial State of Stress
Modeling Hailstone Impact onto Composite Material Panel Under a Multiaxial State of Stress Authors Marco ANGHILERI * LuigiM L CASTELLETTI * Andrea MILANESE * and Andrea SEMBOLONI * Affiliation * Politecnico
More informationAvailable online at ScienceDirect. Procedia IUTAM 10 (2014 )
Available online at www.sciencedirect.com ScienceDirect Procedia IUTAM 10 (2014 ) 285 293 23rd International Congress of Theoretical and Applied Mechanics NanoMechanics foundations and experimental methodologies
More informationMULTISCALE AND MULTILEVEL ANALYSIS OF COMPOSITE STRUCTURES WITH BOLTED JOINTS
MULTISCALE AND MULTILEVEL ANALYSIS OF COMPOSITE STRUCTURES WITH BOLTED JOINTS F.X. Irisarri, J.F. Maire* and N. Carrere ONERA, 9 av. de la Division Leclerc, 930 Châtillon, France francoisxavier.irisarri@onera.fr,
More informationThe Initiation and Growth of Delaminations Induced by Matrix Microcracks in Laminated Composites
International Journal of Fracture, 57, 1 4 199. The Initiation and Growth of Delaminations Induced by Matri Microcracks in aminated Composites J. A. NAIRN and S. HU Department of Materials Science and
More informationCONSTITUTIVE RELATIONS FOR LINEAR ELASTIC SOLIDS
Chapter 9 CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS Figure 9.1: Hooke memorial window, St. Helen s, Bishopsgate, City of London 211 212 CHAPTR 9. CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS 9.1 Mechanical
More informationTransactions on Modelling and Simulation vol 10, 1995 WIT Press, ISSN X
Parameters controlling the numerical simulation validity of damageable composite toughness testing S. Yotte, C. Currit, E. Lacoste, J.M. Quenisset Laboratoire de Genie Meanique  IUT 'A\ Domaine Universitaire,
More informationComputational models of diamond anvil cell compression
UDC 519.6 Computational models of diamond anvil cell compression A. I. Kondrat yev Independent Researcher, 5944 St. Alban Road, Pensacola, Florida 32503, USA Abstract. Diamond anvil cells (DAC) are extensively
More informationUNIT I SIMPLE STRESSES AND STRAINS
Subject with Code : SM1(15A01303) Year & Sem: IIB.Tech & ISem SIDDHARTH GROUP OF INSTITUTIONS :: PUTTUR Siddharth Nagar, Narayanavanam Road 517583 QUESTION BANK (DESCRIPTIVE) UNIT I SIMPLE STRESSES
More informationPoisson s ratio as a sensitive indicator of (fatigue) damage in fibrereinforced plastics
10.1111/j.14602695.2007.01095.x Poisson s ratio as a sensitive indicator of (fatigue) damage in fibrereinforced plastics W. VAN PAEPEGEM, I. DE BAERE, E. LAMKANFI and J. DEGRIECK Ghent University, Department
More informationFinite element analysis of diagonal tension failure in RC beams
Finite element analysis of diagonal tension failure in RC beams T. Hasegawa Institute of Technology, Shimizu Corporation, Tokyo, Japan ABSTRACT: Finite element analysis of diagonal tension failure in a
More informationFREE EDGE DELAMINATION ONSET CRITERION
FREE EGE ELAMINATION ONSET CRITERION G. MARION now, 2, formerl 3, R. HARRY 2, and F. LECUYER MEYSYS, 29 rue J. Rostand, 9873 ORSAY CEEX, FRANCE 2 Laboratoire de Génie Mécanique, IUT Bordeaux I, 3345 TALENCE
More informationDynamic Analysis of a Reinforced Concrete Structure Using Plasticity and Interface Damage Models
Dynamic Analysis of a Reinforced Concrete Structure Using Plasticity and Interface Damage Models I. Rhee, K.J. Willam, B.P. Shing, University of Colorado at Boulder ABSTRACT: This paper examines the global
More informationFailure Mode Predictions in the Compressive Response of Laminated Composites
Structures, Structural Dynamics, and Materials and Colocated Conferences April 811, 2013, Boston, Massachusetts 54th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials Conference AIAA
More information